Symmetryoperations, point groups, space groups and crystal structure


 Geraldine Nichols
 1 years ago
 Views:
Transcription
1 1 Symmetryoperations, point groups, space groups and crystal structure KJ/MV 210 Helmer Fjellvåg, Department of Chemistry, University of Oslo 1994 This compendium replaces chapter 5.3 and 6 in West. Sections not part of the curriculum are enclosed in asterisks (*). It is recommended that the textbooks of West and Jastrzebski are used as supplementary reading material, with special emphasis on illustrative examples. In this compendium illustrative examples (in italics) have been chosen from close packed structures. A few symbols and synonyms are given in Norwegian as information. The compendium contains exercises which will not be explained in the classes. It is recommended to work through the exercises while reading this compendium. Introduction. Condensed phases may be liquids as well as solids. There are fundamental differences between liquids and solids regarding the longrange distribution of atoms. While liquids have long range disorder in a large scale, solids are mainly ordered, i.e. there is regularity in the repetition of structural fragments (atoms and/or groups of atoms) in the 3 dimensional material. Surfaces of solid materials are often somewhat differently organized than the bulk (i.e. the inner part of the material). The atomic (structural) arrangement near the surface will often be different from the bulk arrangement due to surface reconstruction in order to minimize the energy loss associated with complete chemical bonding in all actual directions. Liquids are disordered in bulk, but they often have an ordered surface structure. Solids do not need to display systematic longrange order, i.e. to be crystalline. Some phases can be prepared as amorphous materials, e.g. glasses. They may be made crystallized by a suitable temperature treatment. A few phases exist which are only known in an amorphous state. In order to simplify the description of symmetry relations in atomic arrangements (i.e. the appearance of a structure fragment, molecule or complex) symmetry operations are used. Symmetryoperations like mirroring and rotation are known from everydaylife. If one wishes to describe how structure fragments are repeated (translated) through a solid compound, symmetryoperations which include translation must be used in addition. Symmetrydescriptions of given isolated objects are also known from everydaylife, e.g. a lump of sugar, a dice, a wheel (with an nfold rotation axes for n spokes equally distributed) or a pyramid (with fourfold rotation axis perpendicular to the basis plan).
2 This compendium does not intend to give complete introduction to the basics of symmetry descriptions of solids. That is not the objective of this part of KJMV 210. The text is not written in order to give the reader a perfect and full understanding of crystallography. Instead it will give a simplified picture of the field. The intension of the compendium is to provide a basic knowledge of central issues, so that the reader will be able to draw different structures based on published structural data and available references (International Tables of Crystallography). This will be very useful in later courses concerned with properties of inorganic materials. It is important to realise that there is a close connection between atomic arrangements (structure, chemical bonding) and chemical and physical properties. The chosen examples in the compendium are related to close packing of atoms. The reader is recommended to carefully work through the examples. The unit cell. In the crystalline state there are rules for how structural elements are repeated through the solid. One can identify structural fragments that form the smallest repeating units; by repeating these in 3 dimensions they build the whole material. One can think of the smallest repeating unit as described inside a box. By stacking of the boxes in 3 dimensions a complete description of the structure of the solid material is obtained. Such a box is called a unit cell (enhetscelle). The box is defined by 3 vectors, t 1, t 2 and t 3 [with unit cell volume V = t 1 (t 2 x t 3 )]. The vectors are not necessarily orthogonal. As a starting point there are no conditions on the 3 angles between the vectors, α, β and γ. (i.e. they are not restricted in any way, e.g. to be 90 ). When describing the structure of a solid material in the scientific literature, relevant data for the crystallographic unit cell are given. The unit cell is given by the length of the three axes, a, b and c (unit cell dimensions, unit cell parameters, cell edges; i.e. the lengths of the vectors t 1, t 2 and t 3 ) and the angles α, β and γ. Definition of the angles relative to the axes (t 1, t 2 and t 3 or equivalent a, b and c) is shown in Figure 1. In order to describe the atomic arrangement, one has in addition to defining the shape of the unit cell and also to state where the atoms are in the repeating unit cell. This is done by giving the position of the atoms as coordinates (x,y,z). The atomic coordinates are given as fractions of the unit length of the vectors. Thus position (0,0,0) is the origo of the unit cell, while the point (1,0,0) is moved (t 1,0,0), i.e. one cell edge along the aaxis parallel to t 1. An atom in the corner of the unit cell therefore has the coordinates (0,0,0), while an atom on the centre of the aaxis has the coordinates (1/2,0,0). As a principal rule, any given atom can be transferred to one or more atoms, of the same type and with the same surroundings, within the unit cell by symmetry operations. In order to describe all the atoms in the unit cell it is enough to give the coordinates of a certain part of the atoms along with the necessary symmetry operations. Within a unit cell one often find several atoms of the same kind. If the surroundings of these atoms are identical, the atoms are related by symmetry operations (they are crystallographic equivalent atoms). If the surroundings are more or less different, the difference is signified by using different notations for the atoms, e.g. Cu(1) and Cu(2), where the number in brackets is just numbering of the same type of element. In such cases one would say that Cu(1) and Cu(2) are not crystallographic equivalent atoms. 2
3 3 Figure 1. The definition of relations between angles and axes in unit cells. The unit cell is shown as the box on the left. Example 1 (2dimensional unit cell) A number of simple structures, e.g. for metals and alloys, may be derived from close packing of spheres. Here the atoms are thought to be ideal, non compressible spheres of the same size. Before we look at such 3dimensional structures in details, we will take a closer look at how symmetrynotation can be used to describe close packing in 2dimensions. Then we will add different symmetry operations, still looking at the 2 dimensional model of the structure. Consider a 2dimensional close packing of identical spheres. The spheres are placed as close as possible (i.e. with the least possible space between them). This is shown to the left below. Let us now define a 2dimensional unit cell for the pattern of repeating spheres. We choose the centre of sphere A as origo. (You will get the same unit cell with any other choice of origo, but there will be less symmetry around the origo). The direction and length of the translation vectors (cell edges) must first be determined. Let t 1 be the vector from the centre of sphere A to the centre of sphere 4, and let t 2 be the vector form the centre of sphere A to the centre of sphere 2. The unit cell is completed by translating t 2 so that it starts in the centre of sphere 4 and t 1 to start in the centre of sphere 2. The lengths of the vectors t 1 and t 2 are called a and b. It is obvious that a and b (= 2r; the radius of the sphere). The angle between t 1 and t 2 can easily be calculated by looking at the equilateral triangle that is formed by the centres of three adjacent spheres. The unit cell is therefore defined as a = b and the angle γ = 120 (look above to the right) This 2dimensional packing of spheres is the closest possible, and such layers constitutes the 2dimensional units that are stacked when making 3dimensional close packed structures (notation AB... = hcp, ABC... = ccp, or more unusual and
4 complicated stacking sequence as e.g. ABAC... An... AA...stacking will not be close packed in 3dimensions even though it is built from 2dimensional close packed units). The values of the coordinates (x, y, z) of a point within the unit cell are all between 0 and 1 (look above). Because the unit cell is a repeating unit, any multipla of the unit vectors can be added to or subtracted from any point (x, y, z), in order to get to identical points in other unit cells. The point (x, y, z) or an atom positioned in A in figure 2, e.g. with coordinates (0.21, 0.33, 0.45) is therefore identical to the point B with the coordinates (0.21, 0.33, 1.45) through the translation (x, y, z+1); and C (0.79, 0.33, 0.45) through the translation (x1, y, z); and D (0.79, 1.33, 0.55) through the translation (x1, y+1, z1). A, B, C and D will have identical surroundings in the unit cell and in any given atomic arrangement in a solid material. When atoms are called identical (equivalent) it means that they have absolute identical surroundings in relation to all nearby points/atoms. In example 1, it is seen that the surroundings of e.g. sphere A and sphere 2 are identical. This means that the spheres with centre at the coordinates (0, 0) and (0, 1) are identical. In reality one can view the two spheres as one and the same. Sphere 2 is just sphere A translated one unit translation (the cell edge) along t 2. All the spheres in example 1 are therefore equivalent, and the 2dimensional packing is completely defined by giving a, b and γ together with the information that there is a sphere in origo. Because the unit cell is a repeating unit, a description of the symmetry and the atom coordinates is the unit cell, will describe the symmetry and structure of the solid material. This is of course only true for crystalline phases, where, as mentioned, a systematic longrange order exists. In amorphous materials there are not repeating unit cells. 4 Figure 2: Same point in several unit cells. The chemical composition of a solid material is given by the ratios between the different kind of atoms in the unit cell. If the unit cell is known, it must be possible to make a correct account of the content. One must take in to consideration that one unit is close up against other unit cells and that it shares faces, edges and corners with the surrounding unit cells. Thus, an atom in a unit cell count as 1, whereas an atom on a face counts as ½ (but this is
5 repeated on the opposite unit cell, and together the two half atoms counts as 1); while an atom in a corner counts as 1/8 (but eight corners share a point, so that 8 1/8 = 1); figure 3. As an illustrated, look at Figure 3 where 8 filled symbols are drawn, two open and one hatched. There are the same number of filled, open and hatched symbols in the repeating unit (one of each). 5 Figure 3. Atoms are placed inside the unit cell (hatched), on the faces (open) and at the corners (filled). The unit cells share faces. Exercise 1 Draw a 2dimensional orthogonal unit cell with cell edges a = 3.80 Å and b = 3.90 Å. Place these atoms in the unit cell: Cu(1) in (0, 0) O(1) in (0, 0.5) O(2) in (0.5, 0) Calculate the distance between Cu and O and between Cu and Cu. Check the calculation against what you would expect based on ion/covalent bonding between cupper and oxygen. Such an atomic arrangement is found in 2dimensional sections of high temperature superconductors. Example 2 (3dimensional unit cell; modes of illustration) Imagine taking the 2dimensional layer of spheres as shown in example 1 and putting it right above the exact same layer. The spheres are positioned right on top of one another, and do not fall down the hollows in the layers. It is obvious that this is not a good utilization of the available volume and that the structure is not close packed in 3 dimensions. Stacking of layers is thought continued in such a way that a 3dimensionel object is built. The unit cell of the 2dimensional layer is exactly as seen in example 1. The repeating length in the stacking direction is given by the vector (t 3 ) from the centre of sphere A to sphere A in the next stacking layer. This vector is perpendicular to t 1 and
6 t 2 in the basal plane. The 3dimensional unit cell is therefore a = b c, α= β = 90 and γ = 120. The unit cell can be drawn like this: 6 The structure that arises from such a stacking is said to be a simple hexagonal packing of the type...aa... (NB not a close hexagonal packing). By using the rules for adding up the spheres/atoms will in a unit cell, one finds that the number of atoms is 8 1/8 = 1, i.e. the unit cell contains a formula unit of spheres/atoms; this is given as Z = 1. Note that when one using the notation packing of spheres and looking at rigid touching spheres, this is of course a model, which does not directly describe the properties of the atoms. Atoms (e.g. the noble gases), ions (e.g. Na +, or Cl  ) and metal atoms (e.g. Fe in metallic iron or a iron containing alloy with metallic conductivity) can to a certain degree be seen as spherical. When we draw a crystal structure, where the spheres of the packing model is replaced by atoms, for clarity they are usually drawn so small, that they do not touch one another (look at the figure above). This is done in order to make the figure easier to interpret. When illustrating how much inner volume there is in e.g. a channel in the structure (e.g. a zeolite) the atoms are drawn with a size proportional to covalent, ionic or Van der Waals radius. It is desirable to describe an actual crystal structure with the highest possible symmetry of the structure. For a given structure, it is quite easy to find several unit cells that all fulfil the criteria of repeatability. The crystallographic unit cell must in addition fulfil other criteria. It must:  Display the maximal symmetry of the structure and  At the same time be the smallest repeating unit that does this *In physics (e.g. in theoretical band structure calculations) an other unit cell, the WignerSeitz cell, is often used. This is the smallest repeating unit, but does not show full translational symmetry. When this is used, it is in order to reduce the complexity by including the smallest possible number of atoms. The crystallographic unit cells may contain many formula units, Z (Z is of course an integer, and takes the value of 2 n 3 m, e.g. 1, 2, 3, 6, etc). The WignerSeitz cell is the smallest repeating closed volume around origo (a lattice point). It contains only one lattice point (see space/bravais lattice) and shows the full rotational symmetry of the crystal system (see below). The WignerSeitz cell is constructed by drawing connecting lines from one lattice point to every neighbouring lattice point. Then perpendicular planes are constructed halfway between the lattice points and the surrounded volume that is defined by the planes is the WignerSeitz cell. This volume can have many faces.*
7 Exercise 2: Estimate which of the four following 2dimensional cells fulfil the requirements of a unit cell. 7 E x e r c i s e 3: Draw the NiAs type structure based exclusively on the basis of the following information: a = b = 3.60 Å, c = 5.10 Å, α = β = 90, γ = 120. Ni(1) in ( 0, 0, 0) Ni(2) in ( 0, 0, 0.5) As(1) in ( ⅓, ⅔, ¼) As(2) in ( ⅔, ⅓, ¾) Draw sketches showing the structure seen slightly from the side and as a projection on the abplane. How many formula units (Z) of NiAs are there per unit cell? SI rules say that pm or nm should be used (in stead of Å) to give the unit cell dimensions. What is the unit cell dimensions of NiAs expressed in pm and nm? Calculate the volume of the unit cell and the volume per formula unit. The density of a material is often determined pycnometrically. This returns a measure of the macroscopic density. Porosity (voids, pores between grains/crystallites) and contaminants will contribute to the measured density being smaller than the theoretical value for the material if it was perfect and built in three dimensions from the atomic arrangement found in the unit cell. Using Xray diffraction it is possible to obtain information about the unit cell dimensions. The socalled Xray density is the density calculated from the crystallographic data for the unit cell, i.e. for a perfect material: ρ = m/v = Z FW/V/N A Where FW is the formula weight, N A is Avogadro s number, V is the unit cell volume and Z is the number of formula units in the unit cell. In a number of materials vacancies are found on crystallographic sites, which would be occupied in a perfect case. In other cases additional atoms are situated on nonframework
8 positions (interstitial atoms). From accurate experimental density data it may be possible to estimate the likely defect structure in strongly defect materials (as e.g. defectgenerating solid solution phases, see Chapter 10 in West) if the density for different defect models can be calculated. Crystal systems Exercise 4. Calculate the Xray density of NiAs. Use data for exercise 3. Would you expect the pycnometrically determined density to be larger or smaller than this? NiAs type phases often have significant nonstoichiometry, i.e. the phases may exist with a small or large compositional region. NiAs does not display nonstoichiometry to any significant extent, but let us assume that the phase has interstitial Niatoms, and can be prepared with a composition Ni 1.01 As. In addition let us assume that the unit cell parameters do not change (which they in practice would). Calculate the Xray density for Ni 1.01 As and compare it with the value calculated for NiAs. There are seven different crystal systems. They differ by having different relations between unit cell axes and angles. The relations between the length of the unit cell axes and the angles between them are given in Table 1 and simple unit cells (with one atom in each corner) are shown in Figure 4. (The notation P in Figure 4 indicate that the unit cells are primitive, i.e. they contain only one point or atom, see section on space lattice). 8 Table 1 Relations Crystal system (t1, t2, t3) a = b = c α = β = γ = 90º Cubic a = b c α = β = γ = 90º Tetragonal a b c α = β = γ = 90º Orthorhombic a b c α = γ; β 90º Monoclinic a b c α β γ 90º Triclinic a = b = c α = β = γ 90º Trigonal (Rhombohedral) a = b c α = β; γ = 120º Hexagonal Figure 4. Schematic representation of the unit cells for the seven crystal systems (drawn with one atom in each corner of the unit cell).
9 9 Exercise 5. Give the formula for the volume of (a) a tetragonal, (b) a monoclinic and (c) a hexagonal unit cell expressed by a, b, c, α, β and/or γ. Crystal systems are arranged hierarchically in such a way that the higher crystal system contains at least one symmetry element that the lower system does not contain, see Figure 5. The cubic system is said to have the highest symmetry, and the triclinic the lowest. The symmetry may be seen as increasing from triclinic, via monoclinic, orthorhombic, hexagonal, tetragonal or rhombohedral to the cubic system. Different crystallographic point groups belong to each of the seven different crystal systems (see below). The crystal systems are characterized by having certain symmetry operations. This is further detailed in the section on crystallographic point groups. Figure 5. Hierarchy of crystal systems. The simplest structure types (atomic arrangements) are metals and disordered alloys that crystallize with one of the close packed atomic arrangements, i.e. hexagonal (hcp, hexagonal close packing) or cubic (ccp, cubic close packing. NB! ccp is equivalent to fcc, face centred cubic). As examples could be mentioned that Mg, subgroup III (group 3) (Sc, Y, La) and subgroup IV (group 4) (Ti, Zr, Hf) have hcp structures, while Ni, Pd, Pt, Cu, Ag and Au have ccp structures. Co has both hcp and ccp phases. Hcp phases belong to the hexagonal crystal system, and ccp to the cubic. The simplest anioncation (metal nonmetal) phases mentioned in West s book are based on close packing of anions with the cations in the small holes. For instance the NaCl, CaF 2 , CsCl and zinc blende structure types belong to the cubic crystal system, NiAstype to the hexagonal crystal system, while rutile belong to the tetragonal crystal system. This means that when unit cell dimensions are tabulated for e.g. NaCl, it is sufficient to give the length of the aaxis, as the other relations (a = b = c, angles = 90º) are given by the cubic symmetry. For TiO 2 with the rutile structure, only the a and caxes are given. Example 3 (Assignment of unit cells) Consider the simple hexagonal unit cell, which was described in example 2. From the axes/anglerelations it is seen to satisfy the conditions for a hexagonal unit cell. Therefore the symmetry is said to be hexagonal. In much the same way a simple primitive cubic unit cell may be described by: a = b = c and α = β = γ = 90º. The unit cell is shown below. The cubic unit cell (looking like a cube) has one atom in each corner. It is sufficient to specify that the unit cell is cubic and to give the length of the aaxis. When the structure is drawn as a projection on the ab plane with the radius of the atoms r = a/2, the atoms will touch, and it will be evident that the structure is not close packed, as there are big voids between the spheres.
10 10 Example 4. (Close packing of spheres in three dimensions) Again the starting point is the twodimensional packing of spheres from example 1. Such a layer is close packed. Closer consideration reveals that the spheres touch and are placed like pearls on a string in three directions. Thus, in a close packed layer of spheres there are three close packed directions. If such layers are stacked on top of each other (along the caxis) and systematically shifted with respect to each other in such a way that the spheres of one layer is positioned above the holes of the layer below, a three dimensional close packing of spheres is obtained. This may be best illustrated by drawing the layers on individual transparent foils: Consider one layer. On this layer you draw the twodimensional unit cell described in example 1. The centre of atom A is the origo of the twodimensional unit cell. We now choose this position as the origin of the threedimensional unit cell, which we will derive from stacking of several close packed layers. The Asphere therefore has the position (coordinate) (0,0,0). Also the spheres numbered 2, 3, and 4 in example 1 are described with this position. This is because their positions may be generated by adding to the position (0, 0, 0) multipla of the twodimensional unit cell translations. This means that the position of all the spheres in the layer, which we now will call layer A, are given as (0+n, 0+m, 0) where n and m are integers. Consider the four spheres in the unit cell. Between the spheres there are two indentations, between the 3 spheres A, 4 and 3, and between A, 2 and 3, respectively. We may call the positions which characterize the two indentations B and C. Consider now e.g. the triangle A,4,3 and the point B. By a bit of trigonometry the coordinates (2/3, 1/3) is found for B and (1/3, 2/3) for C. We define two new 2dimentional sheets, named B and C, identical to the A sheet. The B sheet is placed so that there is a sphere right above the B position in the A sheet. The spheres of the B sheet have the coordinates (2/3, 1/3) relative to the chosen origo of the A sheet. In the same way the C sheet is placed so that the spheres have the coordinates (1/3, 2/3) relative to the chosen origo of sheet A. By adding layers on top of each other and using the indentations one obtains a 3dimensional close packing. If the repeating sequence of layer positions is...ab..., it is a hexagonal closest packing (hcp), if the sequence is...abc... it is a cubic close packing (ccp).
11 Any (more complicated) ordering of layers is also a close packing, if there are no layers directly above an identical layer (i.e. there is no...aa...,...bb... or...cc... sequence). The simple ordering sequences are those mentioned above,...ab... and...abc... However in many cases there is very little difference in energy between different ordering sequences for real materials, and the material has many different modifications. The ordering sequences may be complicated (e.g....abcacbcab...). The different ordering variants are called polytypes. These have an identical structure in twodimentions, but some differences in the third dimension, the ordering direction. Polytypes are known in compounds such as Co, SiC, ZnS, ABO 3 and others. 11 schematic ordered stacking of sheets seen from the side (not 100 % correct displacement along the side) Space lattice. The notation space lattice or lattice (romgitter) is a mathematical description of repeating units in solid materials. It is important to realize that a lattice is not the same as a structure. A structure is the atomic arrangement, whereas a lattice is made of mathematical points in space, and these may be translated by certain operations. The similarity between a lattice and the unit cell is striking, especially for the primitive space lattices. The primitive space lattices contain only one point in the repeating unit, and it is placed in the corners of the unit. The different repeating units were described in Unit cells and Crystal systems. There are 7 possibilities, and so there are 7 primitive space lattices. The relations between the translation vectors are also described above. Figure 4 was used to illustrate simple unit cells. The drawings in figure 4 may also represent the primitive space lattices with a lattice point placed in each corner. The primitive lattices are denoted with a P. The primitive rhombohedral is an exception to this rule it is denoted with R. Example 5 (primitive space lattices): Consider the primitive hexagonal space lattice. A (lattice)point (x, y, z) is transferred to equivalent points in the lattice by the translation vectors (t 1, t 2, t 3 ). New (lattice)points have the coordinates (x+nt 1,y+mt 2, z+ot 3 ), where n, m and o are integers. This is drawn in a 2dimentionel projection below. Consider the objects below. They are meant to represent a fragment of a structure. We see that the fragment is repeated in two dimensions. The repetition may be described as (new fragment) = (original fragment) + lattice translation. We choose a random point in one of the fragments, and mark similar points in the other fragments. These
12 points can now be connected by translation vectors t 1 and t 2, which are translation vectors of the 2dimentional, primitive lattice. 12 An absolute requirement to a space lattice is identical surroundings around every single lattice point. This is the starting point to the consideration whether there can be other space lattices than the primitive space lattices described above. It turns out, that all in all there are 14 different lattices which met the requirement. They are called Bravais lattices and are described below. Bravais lattices. It is relatively easy to prove that there are a total of 14 threedimensional lattices which met the criteria of identical surroundings of the lattice points. These are called Bravais lattices, see figure 6. Seven of these are the primitive lattices described above. Figure 6. The 14 Bravais lattices. The primitive Bravais lattices contain only one lattice point. The non primitive Bravais lattices contain more than one lattice point per unit cell (2 or 4), and are called centred lattices:
13 Bodycentred lattice (notation I for Innenzentrierung, new lattice point in a/2 + b/2 + c/2) Facecentred lattice (F, Flächenzentrierung, new lattice points a/2 + b/2 and + a/2 + c/2 and b/2 + c/2) Sidecentred lattice (A, B or C, side centred on only some of the sides, e.g. a/2 + b/2. This is a C side centred lattice, which means that the centring are on the sides normal to the c direction/z axes) The four different types of lattices are illustrated by the orthorhombic Bravais lattices in figure 6. The Bravais lattices matching the crystal systems are given in table 2. Example 6 (Bravais lattices) Close packed, hcp and ccp, have a primitive hexagonal Bravais lattice and a face centred cubic Bravais lattice, respectively (see example 7). The relationship between the ccp packing and the cubic unit cell is discussed in West (see figure 7.5) but the relationship may be somewhat difficult to see. The close packed layers in the ccp structure lies perpendicular to the space diagonals in the cubic cell. The cubic unit cell has atoms placed in the corners and in the center of all the faces. If we neglect that there are atoms in the cell and replace them with mathematical points, it is clear that it is a cubic Bravais lattice with F centring. If an atom is placed at every lattice point, the face centred cubic structure is reached. This is known as fcc. This is also identical to ccp. For a fccmetal Z = 4. Table 2: Crystal system Bravais lattice Z Cubic P 1 I 2 F 4 Tetragonal P 1 I 2 Orthorhombic P 1 I 2 C 2 F 4 Monoclinic P 1 C 2 Triclinic P 1 Rombohedral R 1 Hexagonal P 1 The centred Bravais lattices may also be represented by smaller primitive unit cells. These will however not show the highest symmetry of the system, which is a requirement for a crystallographic unit cell. See figure 7. Exercise 6: Show how the cubic FBravais lattice fulfils the requirements of a lattice (consider the surroundings of every lattice point). 13
14 Exercise 7: Draw a tetragonal P lattice. Place an extra lattice point in ½, ½, 0, i.e. make a C centring of the lattice. Show that a tetragonal C lattice does not exist as such, i.e., that it is equivalent to (another) P lattice. Brasvais lattices define the way a lattice point (ore a fragment of a structure, see example 5) is transferred to identical points (ore fragments). A crystal structure can therefore be described as structure = lattice + basis where the basis is made of the repeating structure fragment with a number of atoms with coordinates (x i, y i, z i ). 14 Figure 7. Relationship between primitive cells and F, I and C centred cells. Some simple crystal structures are shown in Figure 8. From these it is possible to say what type of Bravais lattice the different structure types has. E.g. CsCl type structure has a Bravais lattice Pcubic, NaCl and CaF 2 type have a Fcubic, NiAs type is Phexagonal, whereas bcc (metal) has a Icubic Bravais lattice. How this is seen is explained in example 7. Figure 8. Schematic representation of NaCl, CaF 2 , CsCl and bcc type crystal structure. The symbols below the figures are space group notation. Example 7 (Bravais lattice): In this example we take a closer look at the CsCl type structure and hcp. In CsCl (figure 8) the black spheres form a primitive cubic lattice (a=b=c, angles = 90º). The sphere in the centre is of another type and has nothing to do with the lattice of the black spheres. If several unit cells are drawn beside each other, it is possible to see which repeating rules that can be applied to the open spheres. You will find that the repeating unit is an identical cubic box with the same edge as the one of the black spheres. The Bravais lattice is the same, but because the spheres are different, they both are part of the basis of the structure; i.e. the CsCl type structure has a cubic P lattice with Cs in (0, 0, 0) and Cl in (½, ½, ½). This can be seen as: CsCl type structure = cubic Plattice + basis [Cs in (0, 0, 0) and Cl in ((½, ½, ½)]
15 15 It is also easy to show that the hcp structure has a primitive hexagonal Bravais lattice. Look at the figure below. The open spheres represent sheet A, the black sheet B, as in previous examples. Four unit cells (with a sphere A in origo) are marked with a full line. Consider now the 4 B spheres. They define a unit cell as well (dotted line) which in shape and size is identical to the one defined by the Aspheres. The only difference is that the Bcells origo has been moved to (2/3, 1/3). In order to describe the hcp structure, the Bravais lattice can be said to be hexagonal primitive and basis to be two atoms in respectively (0, 0, 0) and (2/3, 1/3, 1/2); i.e. hcp type structure = hexagonal Plattice + basis [M in (0, 0, 0) and M in (2/3, 1/3, 1/2)] A better description is given in example 9, where symmetry elements are considered as well. Symmetry operations Exercise 8: Draw the structure of the anioncation compound AB on the basis of the following information: The Bravais lattice is Fcubic Basis: A atom in (0, 0, 0) and B atom in (1/2, 0, 0) What is the name of this type of structure? Exercise 9: Ni has a cubic face centred structure, known as fcc, i.e. face centred cubic with basis: Ni in (0, 0, 0). The cell edge is 351 pm. Calculate the radius of the Ni spheres (metallic radius). Calculate the density of Ni. In the following we will consider symmetry operations that can be used to describe isolated objects, e.g. a molecule in gas phase. The requirement of a symmetry operation is that when it operates (is used) on an atom with a set of atomic coordinates (x, y, z), an atom of the same type and with identical surroundings is created, but with the coordinates (x, y, z ). These are the symmetry elements which exist:  Identity, that is (x, y, z) is transferred to itself (x, y, z). This symmetry element is included, because it is a requirement in the definition of a group in group theory, which is the mathematical tool used in symmetry considerations.  Inversion, that is (x, y, z) is translated to (x, y, z). If an object has this symmetry element, it is said to be centrosymmetric (det er sentrosymmetrisk).
16  Rotation axis, a rotation axis is two fold, three fold etc. A nfold axis rotate an object 360º/n.  Mirror plane which places the object laterally reversed (mirror image) as far behind the mirror plane as it was in front. E.g. an xymirror plane (i.e. the xy plane is thought to be the plane of the mirror) transfers a point (x, y, z) to (x, y, z). Inversion symmetry and mirror planes both transfers a right handed object to a left handed object (like a mirror image; this is shown by writing a comma (,) in the circles, as shown in figure 9. The effect of these symmetry operations is schematically shown with hands in figure 9. The nomenclature (symbols) are also shown. 16 Figure 9: Inversion, reflection and two fold axes. The effect of the operations is shown with hands. The use of symbols is further described in point groups. The origin of the symmetry operations and the coordinate system are chosen so as to reveal the highest possible symmetry. Two sets of nomenclature are used to indicate symmetry operations. Schönflies nomenclature is often used in spectroscopy, whereas HermannMauguin nomenclature is used in crystallography (description of structure). The notation is different, but the operations are of course the same, see Table 3. Table 3 Symmetry operation Schönflies symbol HermannMauguin symbol Identity E or I I Inversion i (centro symmetric) Rotation axis C n (n=fold) n Mirror plane σ h, σ v m (reflection) σ h and σ v are the notation for the horizontal and the vertical mirror plane respectively (defined relative to the main rotation axis. Exercise 10: Which symmetry operations can you identify for the following objects: (a) H 2 O (b) NH 3 (c) CO 2 (d) CH 4 (e) a d xy orbital There are also combined symmetry operations, which means that two symmetry operations are performed right after each other and thus the intermediate state is not considered. Rotationinversion axes are used in crystallography [rotationinversion axes are denoted as n, often expressed as n ], i.e. a nfold rotation is done followed by an inversion. In the _ 1
17 Schönflies notation rotationinversion axes are denoted S n. Some examples of such symmetry operations are shown in figure 10. Exercise 11: The tetrahedron belongs to the group of objects with a symmetry in the cubic system. Compare the 4fold rotation axes in a cube and in a tetrehedra. 17 Figure 10: Symmetry operations 4, 6, 4 & 6. Example 8 (Rotation axes, crystal system) Let us consider hcp close packing. Let us first consider a 2dimensional A sheet, and choose origo to be in the centre of a chosen sphere. We can now evaluate the nfold rotation axis perpendicular to the close packed sheet. By a rotation of 60º the picture is identical, i.e. we have a 360º/60º = 6fold rotation axis. This is characteristic for the hexagonal crystal system, cf. Table 5. If we construct an AB packing, we see that the 6fold axes is not preserved, but in each sheet there are points with a 6fold symmetry. This is discussed further in the paragraph on glide planes and screw axes. Example 9 (Choise of origo, center of symmetry): We consider at a projection of the hcp structure onto the ab plane: Let us evaluate if this unit cell has an inversion center, i.e. it is centro symmetric. In this case all atomic coordinates, were given relative to the centre of symmetry placed in origo, must be transferred to identical coordinates for atoms by the inversion operation (x i, y i, z i ) (x i, y i, z i ) If the origin chosen at the centre of an Aatom (open symbol, solid unit cell) we see that there are no centro symmetric surrounding A. For atom B with coordinates (2/3, 1/3, 1/2) there are no identical B or Aatoms (A and B are identical atoms/spheres)
18 with coordinates (1/3, 2/3, 1/2) = (2/3, 1/3, 1/2) = (2/3 +1, 1/3 +1, 1/2+1); see solid arrow. The apparent lack of centro symmetry is actually due to the fact that we have chosen the wrong point as the centre of symmetry. Let us choose the point (1/3, 2/3, 1/4) as origo, which is assumed to be a centre of symmetry. First the coordinates in sheet A and B must be transformed to (01/3, 02/3, 01/4) = (2/3, 1/3, 3/4) and (2/3 1/3, 1/3 2/3, 1/2 1/4) = (1/3, 2/3, 1/4), respectively. It is now easy to see that a centre of symmetry relates sheet A and sheet B, cf. the dotted arrow. The hcp structure is therefore centro symmetric. The unit cell with a center of symmetry in origo is dotted. A closer look at the figure reveals that there are more points, which are center of symmetry than (0, 0, 0). 18 Point groups. A point group is described by a characteristic assembly of symmetry operations. A certain number of symmetry operations with defined geometrical relations among themselves can be found for any given object. The object is said to have symmetry described by the given point group. Different objects which have different symmetry will therefore be described with different point groups. All symmetry elements present refer to a common point, the origo. *A point group must fulfil the mathematical requirements of a group:  The product of two operations is another operation in the group  The identity element (I) is present  The existence of an inverse operator RR 1 = 1  Associative multiplication of operations* The point groups have different notation in Schönflies and HermannMauguin nomenclature. In Schönflies nomenclature there are point groups such as C nv, C nh, D nh, T d, O h etc, where n is the highest number of rotation axes present and v is the vertical mirror plane, which is only mentioned if there are no horizontal mirror planes (h). If there are twofold axes perpendicular to the highest rotation axes, the point group is D nh. T is a tetrahedral and O is an octahedral point group (cubic crystal system). In the HermannMauguin nomenclature similar information is given. The highest rotation axis is given first. E.g. a point group with only a twofold rotation axes is denotated 2. C 2h (Schönflies) is notated 2/m, where the slash indicate that the mirror plane is perpendicular to the twofold axis. In the following only the HermannMauguin nomenclature is used. The two types of nomenclature are compared for a number of point groups in Table 4. Table 4. HermannMauguin nomenclature: /m 3 4/m 6/m mmm 3 m 4/mmm 6/mmm m3 m3m Schönflies nomenclature: C 1 C 2 C 3 C 4 C 6 D 2 D 3 D 4 D 6 T O C i C 2h S 6 C 4h C 6h D 2h D 3d D 4h D 6h T h O h
19 19 Example 10 (point symmetry): Consider a small section of the close packing in twomensions in example 1 by choosing one sphere and the surrounding six. First we define the directions by letting the a and baxes be in the basal plane as shown in example 1. We let the caxis be perpendicular to the abplane. The relations between the axes are those required in the hexagonal crystal system. We observe a 6fold rotation axis runs through the central sphere and parallel to the caxis. The basal plane is a mirror plane. Therefore the HermannMauguin symbol must be 6/m. The full symbol is larger because all information on the symmetry relations along the axes in the basal plane must be given as well. This is described in the second part of the example below. Exercise 12. Give the Schönflies and HermannMauguin symbols for point groups with the following symmetry elements: (a) a fourfold rotation axis (b) identity and an inversion axis (c) a fourfold rotation axis and a mirror plane perpendicular to the rotation axis. Exercise 13: Which symmetry elements can you identify in the point groups: (a) 1 (b) 3 (c) 6/m (d) 4/m For isolated objects there is no limit on the n fold of a rotation axis. Therefore one can imagine an infinite number of point groups, but only a few of these are found frequently in real objects. A fivefold rotation axis exists e.g. in an isolated flat C 5 H 5 molecule. Global fivefold symmetry cannot appear in ordered, threedimensional crystalline phases. On the other hand it is possible to observe units with a local fivefold symmetry in solid materials, even though it is not possible to fit 5fold symmetry into a repeating lattice (see below). The point group symbol tells which symmetry elements are essential to the point group (these may create other symmetry elements by being used on each other). Consider e.g. the point group 2/m. The symbol reveals that there is a twofold rotation axis and a horizontal mirror plane. Because these elements are both present, the inversion element is automatically present too, figure 11. Thus, 2/m is a centro symmetrical point group. All in all the point group 2/m contain the symmetry operations. Identity, twofold rotation axis, horizontal mirror plane and inversion. Figure 11. Structure fragment with point symmetry 2/m.
20 20 Those point groups which contain an inversion element are considered centro symmetrical. Certain properties in a material depend on the symmetry, e.g. the existence of electric dipoles, optic activity, pyro and piezoelectricity. The last two are discussed in chapter 15 in West (not part of the curriculum). Exercise 14: Explain why a molecule with a permanent electric dipole (i.e. the molecule has a dipole moment) cannot be centro symmetric. Can a material built by hcppacking display permanent polarization (i.e. have a total sum of dipole moments that is not zero)? So far we have limited the description to cases with one rotation axis and one mirror plane (vertical or horizontal). If the description is extended to include also symmetry relations in orthogonal directions, the result is a number of new point groups. One can e.g. imagine a point group with three twofold rotation axes, in the directions x, y and z in a cartesian coordinate system. This point group is called 222 (orthorhombic system) where all the symbols (the 2 s) describe the symmetry relations in the orthogonal directions. The combined point group symbols e.g. mm2 are interpreted following certain rules. For example the first symbol for orthorhombic and tetragonal point groups describes the symmetry along the zaxis (which is thereby chosen to have the highest rotation axis in the tetragonal crystal system), the next symbol describes the relations in a perpendicular direction (e.g. the yaxis) and in the orthorhombic system the last symbol describes the relations in the third direction, whereas in the tetragonal system it describes the symmetry in the [110] direction. More specialized rules for symbol, 2 and 3 must be used for trigonal, hexagonal and cubic point groups. Example 10 (point symmetry, continued): In the hexagonal crystal system the first part of the combined point group symbol describes the symmetry conditions along the caxis, the next the conditions along the a and baxes, and the third the conditions along a direction perpendicular to the a and baxes. If we look at the isolated object (1+6 spheres) we see that the aaxis is a twofold rotation axis with a perpendicular mirror plane, i.e. with the symbol 2/m. We also note that perpendicular to the aaxis there is another twofold rotation axis with a perpendicular mirror plane. The correct point group symbol is therefore 6/m2/m2/m. Exercise 15: Consider the flat molecule transdichloroethen C 2 H 2 Cl 2. Draw the molecule in the xyplane (let the zdirection be the direction with the twofold axis). Identify the symmetry operations I, C 2 z, σ h xy and i (in Schönflies nomenclature). What are these called in HermannMauguin nomenclature? Explain why the point group symbol is C 2h (Schönflies). How would you describe the point group with crystallographic nomenclature? Show that the assembly of symmetry elements fulfils the requirements of a group. The point groups are classified under the different crystal systems. For a given crystal system certain characteristic symmetry elements can be identified, see Table 5. Note that the cubic crystal system is not characterized by the presence of fourfold axes, but by the existence of four threefold axes.
WHICH SCORING RULE MAXIMIZES CONDORCET EFFICIENCY? 1. Introduction
WHICH SCORING RULE MAXIMIZES CONDORCET EFFICIENCY? DAVIDE P. CERVONE, WILLIAM V. GEHRLEIN, AND WILLIAM S. ZWICKER Abstract. Consider an election in which each of the n voters casts a vote consisting of
More informationProperties of Electrons, their Interactions with Matter and Applications in Electron Microscopy
Properties of Electrons, their Interactions with Matter and Applications in Electron Microscopy By Frank Krumeich Laboratory of Inorganic Chemistry, ETH Zurich, VladimirPrelogWeg 1, 8093 Zurich, Switzerland
More informationFoundations of Data Science 1
Foundations of Data Science John Hopcroft Ravindran Kannan Version /4/204 These notes are a first draft of a book being written by Hopcroft and Kannan and in many places are incomplete. However, the notes
More informationFoundations of Data Science 1
Foundations of Data Science John Hopcroft Ravindran Kannan Version 2/8/204 These notes are a first draft of a book being written by Hopcroft and Kannan and in many places are incomplete. However, the notes
More informationHighDimensional Image Warping
Chapter 4 HighDimensional Image Warping John Ashburner & Karl J. Friston The Wellcome Dept. of Imaging Neuroscience, 12 Queen Square, London WC1N 3BG, UK. Contents 4.1 Introduction.................................
More informationThe Set Data Model CHAPTER 7. 7.1 What This Chapter Is About
CHAPTER 7 The Set Data Model The set is the most fundamental data model of mathematics. Every concept in mathematics, from trees to real numbers, is expressible as a special kind of set. In this book,
More informationGroup Theory via Rubik s Cube
Group Theory via Rubik s Cube Tom Davis tomrdavis@earthlink.net http://www.geometer.org ROUGH DRAFT!!! December 6, 2006 Abstract A group is a mathematical object of great importance, but the usual study
More informationOPRE 6201 : 2. Simplex Method
OPRE 6201 : 2. Simplex Method 1 The Graphical Method: An Example Consider the following linear program: Max 4x 1 +3x 2 Subject to: 2x 1 +3x 2 6 (1) 3x 1 +2x 2 3 (2) 2x 2 5 (3) 2x 1 +x 2 4 (4) x 1, x 2
More informationHow to Read MTF Curves
How to Read MTF Curves by H. H. Nasse Carl Zeiss Camera Lens Division December 28 Preface The rules of optics are complex and nasty! This is a nice, honest sentence from an internet discussion about How
More informationAll of mathematics can be described with sets. This becomes more and
CHAPTER 1 Sets All of mathematics can be described with sets. This becomes more and more apparent the deeper into mathematics you go. It will be apparent in most of your upper level courses, and certainly
More informationAn Introduction to Tensors for Students of Physics and Engineering
NASA/TM 2002211716 An Introduction to Tensors for Students of Physics and Engineering Joseph C. Kolecki Glenn Research Center, Cleveland, Ohio September 2002 The NASA STI Program Office... in Profile
More informationDie Naturwissenschaften 1935. Volume 23, Issue 48. The Present Status of Quantum Mechanics By E. Schrödinger, Oxford.
Die Naturwissenschaften 1935. Volume 23, Issue 48. The Present Status of Quantum Mechanics By E. Schrödinger, Oxford. Contents 1. The Physics of Models. 2. The Statistics of Model Variables in Quantum
More informationHow many numbers there are?
How many numbers there are? RADEK HONZIK Radek Honzik: Charles University, Department of Logic, Celetná 20, Praha 1, 116 42, Czech Republic radek.honzik@ff.cuni.cz Contents 1 What are numbers 2 1.1 Natural
More informationNotes on finite group theory. Peter J. Cameron
Notes on finite group theory Peter J. Cameron October 2013 2 Preface Group theory is a central part of modern mathematics. Its origins lie in geometry (where groups describe in a very detailed way the
More informationCS488/688. Sample Exam Questions
CS488/688 Sample Exam Questions University of Waterloo School of Computer Science Computer Graphics Lab January 14, 2015 This is a set of questions covering the course material. They have been asked on
More informationIndexing by Latent Semantic Analysis. Scott Deerwester Graduate Library School University of Chicago Chicago, IL 60637
Indexing by Latent Semantic Analysis Scott Deerwester Graduate Library School University of Chicago Chicago, IL 60637 Susan T. Dumais George W. Furnas Thomas K. Landauer Bell Communications Research 435
More informationIntroduction to Group Theory with Applications in Molecular and Solid State Physics
Introduction to Group Theory with Applications in Molecular and Solid State Physics Karsten Horn FritzHaberInstitut der MaxPlanckGesellschaft 3 84 3, email horn@fhiberlin.mpg.de Symmetry  old concept,
More informationElementary Topology Problem Textbook. O. Ya. Viro, O. A. Ivanov, N. Yu. Netsvetaev, V. M. Kharlamov
Elementary Topology Problem Textbook O. Ya. Viro, O. A. Ivanov, N. Yu. Netsvetaev, V. M. Kharlamov Dedicated to the memory of Vladimir Abramovich Rokhlin (1919 1984) our teacher Contents Introduction xi
More informationMeasurement. Stephanie Bell. Issue 2
No. 11 Measurement Good Practice Guide A Beginner's Guide to Uncertainty of Measurement Stephanie Bell Issue 2 The National Physical Laboratory is operated on behalf of the DTI by NPL Management Limited,
More informationhow to use dual base log log slide rules
how to use dual base log log slide rules by Professor Maurice L. Hartung The University of Chicago Pickett The World s Most Accurate Slide Rules Pickett, Inc. Pickett Square Santa Barbara, California 93102
More information2 Basic Concepts and Techniques of Cluster Analysis
The Challenges of Clustering High Dimensional Data * Michael Steinbach, Levent Ertöz, and Vipin Kumar Abstract Cluster analysis divides data into groups (clusters) for the purposes of summarization or
More informationIf A is divided by B the result is 2/3. If B is divided by C the result is 4/7. What is the result if A is divided by C?
Problem 3 If A is divided by B the result is 2/3. If B is divided by C the result is 4/7. What is the result if A is divided by C? Suggested Questions to ask students about Problem 3 The key to this question
More informationCommon Core State Standards for. Mathematics
Common Core State Standards for Mathematics Table of Contents Introduction 3 Standards for Mathematical Practice 6 Standards for Mathematical Content Kindergarten 9 Grade 1 13 Grade 2 17 Grade 3 21 Grade
More informationChapter 3. The Structure of Matter and. Review Skills
Chapter 3 The Structure of Matter and the Chemical Elements One doesn t discover new lands without consenting to lose sight of the shore for a very long time. Andre Gide French Novelist and Essayist n
More informationA Tutorial on Support Vector Machines for Pattern Recognition
c,, 1 43 () Kluwer Academic Publishers, Boston. Manufactured in The Netherlands. A Tutorial on Support Vector Machines for Pattern Recognition CHRISTOPHER J.C. BURGES Bell Laboratories, Lucent Technologies
More informationTHE PROBLEM OF finding localized energy solutions
600 IEEE TRANSACTIONS ON SIGNAL PROCESSING, VOL. 45, NO. 3, MARCH 1997 Sparse Signal Reconstruction from Limited Data Using FOCUSS: A Reweighted Minimum Norm Algorithm Irina F. Gorodnitsky, Member, IEEE,
More information1 Sets and Set Notation.
LINEAR ALGEBRA MATH 27.6 SPRING 23 (COHEN) LECTURE NOTES Sets and Set Notation. Definition (Naive Definition of a Set). A set is any collection of objects, called the elements of that set. We will most
More informationJust want the standards alone? You can find the standards alone at http://corestandards.org/thestandards
4 th Grade Mathematics Unpacked Content For the new Common Core State Standards that will be effective in all North Carolina schools in the 201213 school year. This document is designed to help North
More informationPRINCIPAL COMPONENT ANALYSIS
1 Chapter 1 PRINCIPAL COMPONENT ANALYSIS Introduction: The Basics of Principal Component Analysis........................... 2 A Variable Reduction Procedure.......................................... 2
More informationRevisiting the Edge of Chaos: Evolving Cellular Automata to Perform Computations
Revisiting the Edge of Chaos: Evolving Cellular Automata to Perform Computations Melanie Mitchell 1, Peter T. Hraber 1, and James P. Crutchfield 2 In Complex Systems, 7:8913, 1993 Abstract We present
More information